Fabrication of low-temperature solid oxide fuel cells with a nanothin protective layer by atomic layer deposition
© Ji et al.; licensee Springer. 2013
Received: 18 July 2012
Accepted: 4 January 2013
Published: 23 January 2013
Anode aluminum oxide-supported thin-film fuel cells having a sub-500-nm-thick bilayered electrolyte comprising a gadolinium-doped ceria (GDC) layer and an yttria-stabilized zirconia (YSZ) layer were fabricated and electrochemically characterized in order to investigate the effect of the YSZ protective layer. The highly dense and thin YSZ layer acted as a blockage against electron and oxygen permeation between the anode and GDC electrolyte. Dense GDC and YSZ thin films were fabricated using radio frequency sputtering and atomic layer deposition techniques, respectively. The resulting bilayered thin-film fuel cell generated a significantly higher open circuit voltage of approximately 1.07 V compared with a thin-film fuel cell with a single-layered GDC electrolyte (approximately 0.3 V).
KeywordsAtomic layer deposition Protective layer Thin-film solid oxide fuel cell Yttria-stabilized zirconia Gadolinium-doped ceria Anodic aluminum oxide
Solid oxide fuel cells (SOFCs) normally operate at considerably high temperatures (>700°C) to facilitate ionic charge transport and electrode kinetics [1, 2]. Encountered by issues such as limited material selection and poor cell durability, many researchers have tried to reduce the operating temperature [3–5]. However, lower operating temperature led to a significant sacrifice in energy conversion efficiency due to the resulting increase in ohmic and activation losses .
There are roughly two ways to minimize the ohmic loss surging at lower operating temperatures. One is to reduce the thickness of the electrolyte, and the other is to synthesize materials with higher ionic conductivities. First, the strategy to reduce in electrolyte thickness has been carried out by many research groups [6–10]. Shim et al. demonstrated that a fuel cell employing a 40-nm-thick yttria-stabilized zirconia (YSZ) can generate a power density of 270 mW/cm2 at 350°C , while Kerman et al. demonstrated 1,037 mW/cm2 at 500°C from a 100-nm-thick YSZ-based fuel cell . Another approach of minimizing ohmic loss is using electrolytes with higher ionic conductivities. Gadolinium-doped ceria (GDC) has been considered as a promising electrolyte material due to its excellent oxygen ion conductivity at low temperatures [13, 14]. However, the tendency of GDC being easily reduced at low oxygen partial pressures makes its usage as a fuel-cell electrolyte less attractive because the material will have a higher electronic conductivity as it is reduced. For this reason, many studies have been performed to prevent electronic conduction through GDC film by placing an electron-blocking layer in the series [15–17]. Liu et al. demonstrated the electron-blocking effect of a 3-μm-thick YSZ layer in a thin-film fuel cell with a GDC/YSZ bilayered electrolyte . If the GDC electrolyte thickness was reduced down to a few microns, another problem emerges, i.e., oxygen gas from the cathode side starts to permeate through the thin GDC electrolyte [13, 19]. For the reasons mentioned, the application of a protective layer is essential for GDC-based thin-film fuel cells. Recently, Myung et al. demonstrated that a thin-film fuel cell having a 100-nm-thick YSZ layer deposited by pulsed laser deposition onto a 1.4-μm-thick GDC layer actually prevented both the reduction of ceria at low oxygen partial pressures and oxygen permeation across the GDC thin layer . For the development of large-scale thin-film fuel cells, an anodic aluminum oxide (AAO) template has been considered as their substrate due to its high scalability potential. However, commercially available AAO templates have a considerably rough surface unlike silicon-based substrates, which have been used for conventional thin-film fuel cells. For this reason, atomic layer deposition (ALD) technique was employed to deposit a highly conformal and dense YSZ layer to minimize uncontrolled pinholes and/or morphological irregularities.
In this report, we demonstrate a prototypical, AAO-supported thin-film fuel cell with a bilayered electrolyte comprising a GDC film and a thin protective YSZ layer. The radio frequency (RF)-sputtered GDC layer with excellent oxygen ion conductivity is used as the primary electrolyte layer, while the YSZ layer deposited by ALD technique prevents the reduction of ceria at low oxygen partial pressure and oxygen permeation across the GDC thin layer. To investigate the effect of ALD YSZ layer as a protective layer, the electrochemical performance of a GDC/YSZ bilayered thin-film electrolyte fuel cell is compared with that of a single-layered GDC-based thin-film fuel cell.
Chemical composition of thin films was analyzed by X-ray photoelectron spectroscopy (XPS) (AXIS Hsi, Kratos Analytical, Ltd., Manchester, UK). Possible surface contamination was eliminated by 150 eV of Ar-ion etching for 30 s prior to XPS analysis. The microstructure of thin films was investigated using focused ion beam and field emission scanning electron microscopy (FE-SEM) (Quanta 3D FEG, FEI Company, Hillsboro, OR, USA), and a few nanometer-thick Pt layer was coated on samples to prevent thin films from being etched by FE-SEM imaging.
A test cell was attached to a custom-made hydrogen feeding chamber using a ceramic adhesive (CP4010, Aremco Products, Inc., Briarcliff Manor, NY, USA) and heated to 450°C using a halogen heating system. Dry H2 gas with a mass flow of 25 sccm was supplied to the anode side, and cathode was exposed to atmospheric environment. Anode was connected to a silver wire, and cathode was contacted by a hardened steel probe. Polarization of thin-film fuel cells was analyzed using an electrochemical testing system (1287/1260, Solartron Analytical, Hampshire, UK).
Results and discussion
Thin-film electrolyte fabrication
Subsequently, YSZ thin films were fabricated by co-deposition of zirconia and yttria. Zirconia was deposited prior to yttria deposition. Yttria mole fraction in the ALD YSZ thin-film was controlled by changing the ratio of deposition cycles for zirconia and yttria. The yttria mole fraction is widely known to determine oxygen ion conductivity in the YSZ, and 8% mole yttria was reported to render the maximum oxygen ion conductivity . When the ratio of zirconia and yttria ALD cycle was 7:1, the atomic concentrations of the YSZ thin-film were as follows: Zr 3d = 24.2%, Y 3d = 3.6%, and O 1s = 72.1%, which were also determined by an XPS analysis. The Y2O3 mole fraction, x, in the YSZ chemical formula of (ZrO2)1−x(Y2O3) x was approximately 0.07. In the case of the YSZ thin-film, the XPS spectra corresponding to an under-stoichiometric ZrO2 did not appear, unlike those in the zirconia thin-film.
Design of AAO-supported GDC/YSZ bilayered thin-film fuel cell
A commercial AAO (Synkera Technology Inc., Longmont, CO, USA) template with an 80-nm pore and a 100-μm height was used as the substrate to leverage their high density of nanopores and resulting electrochemical reaction sites [28, 29]. Pt electrode was fabricated by a commercial sputter (A-Tech System Ltd.). Pt with 99.9% purity was used as the Pt target, and the T-S distance was 100 mm. The deposition was conducted at room temperature, and the direct current power was set to 200 W. The Pt anode was deposited on the AAO template in an area of 10 × 10 mm2. Dense Pt anodes were deposited at a 5-mTorr Ar pressure, having the growth rate of approximately 60 nm/min. Subsequently, YSZ and GDC electrolytes with an area of 9 × 9 mm2 were deposited on the Pt anode. The critical thickness ratio of the YSZ layer to the GDC layer to prevent the reduction of ceria, which was determined considering the distribution of oxygen activity through the thickness of a bilayer, was reported to be approximately 10−4 at 800°C and was expected to decrease further at lower temperatures . For this reason, the required minimum thickness of the YSZ layer for electron blockage, if the thickness of GDC layer is 420 nm, is only approximately 0.4 Å. However, a much thicker YSZ film (40 nm) was deposited on the anode side to compensate the rough morphological variations of the Pt-coated AAO surface. The GDC layer, which was 420-nm thick, was then deposited on the YSZ layer. Oxygen reduction reaction happening at the cathode is widely known to cause a significantly greater activation loss compared with the hydrogen oxidation reaction occurring at the anode . In order to facilitate cathode reaction, a porous Pt cathode was prepared by depositing at a much higher Ar pressure of 90 mTorr than that used for anode deposition (5 mTorr Ar). The cathode thickness was approximately 200 nm. The growth rate still remained at approximately 60 nm/min. The Pt cathode, which effectively determines the nominal area of active cell, was deposited using a mask with 1 × 1 mm2 openings.
Electrochemical evaluation of thin-film fuel cells
In this study, we implemented and suggested a promising feasibility of a thin-film low-temperature SOFC using a bilayered electrolyte configuration on the AAO platform. GDC has suffered from its chemical instability and the resulting electronic leakage under a reduction environment. In a thin-film configuration for securing a decent oxygen ion conductivity even at low temperatures (as an LT-SOFC), oxygen permeation through the GDC film became problematic as well. This paper reports that an insertion of a very thin ALD YSZ layer between the anode Pt and the GDC electrolyte significantly improved the electrochemical performance of a cell. At 450°C, a thin-film fuel cell with 850-nm-thick GDC electrolyte showed an OCV of approximately 0.3 V and a power density of approximately 0.01 mW/cm2. On the other hand, a thin-film fuel cell with a bilayered electrolyte consisting of a 40-nm-thick YSZ and a 420-nm-thick GDC reached an OCV of approximately 1.07 V and a power density of approximately 35 mW/cm2. From these results, it was confirmed that the YSZ layer successfully acted as a protective layer. The cell performance is expected to further improve through the microstructural optimization of electrode interfaces and adjustment of chemical compositions of each film.
While the fully functional YSZ layer presented here is already very thin (40 nm), there are good chances of reducing the thickness even further considering that a theoretical approach predicted an YSZ-to-GDC thickness ratio of 0.01% would suffice to guarantee electron blockage .
SJ and IC are students in the Graduate School of Convergence Science and Technology, Seoul National University. YHL, JP, and JYP are graduate students in the School of Mechanical and Aerospace Engineering, Seoul National University. MHL is a professor in the School of Engineering at the University of California, Merced. SWC is a professor in the School of Mechanical and Aerospace Engineering, Seoul National University.
This work was supported by the Global Frontier R&D Program in the Center for Multiscale Energy System funded by the National Research Foundation under the Ministry of Education, Science and Technology, Korea (2011–0031569).
- O’Hayre R, Cha SW, Colella W, Prinz FB: Fuel Cell Fundamentals. John Wiley & Sons, New York; 2006.
- Yamamoto O, Taeda Y, Kanno R, Noda M: Perovskite-type oxides as oxygen electrodes for high temperature oxide fuel cells. Solid State Ion 1987, 22: 241. 10.1016/0167-2738(87)90039-7View Article
- Lee C, Bae J: Oxidation-resistant thin film coating on ferritic stainless steel by sputtering for solid oxide fuel cells. Thin Solid Films 2008, 516: 6432. 10.1016/j.tsf.2008.02.045View Article
- Yokokawa H, Tu H, Iwanschitz B, Mai A: Fundamental mechanisms limiting solid oxide fuel cell durability. J Power Sources 2008, 182: 400. 10.1016/j.jpowsour.2008.02.016View Article
- Hibino T: A low-operating-temperature solid oxide fuel cell in hydrocarbon-air mixtures. Science 2031, 2000: 288.
- Muecke UP, Beckel D, Bernard A, Bieberle-Hütter A, Graf S, Infortuna A, Müller P, Rupp JLM, Schneider J, Gauckler LJG: Micro solid oxide fuel cells on glass ceramic substrates. Adv Funct Mater 2008, 18: 3158. 10.1002/adfm.200700505View Article
- Fabbri E, Pergolesi D, D’Epifanio A, Bartolomeo ED, Balestrino G, Licoccia S, Traversa E: Design and fabrication of a chemically-stable proton conductor bilayer electrolyte for intermediate temperature solid oxide fuel cells (IT-SOFCs). Energy Environ Sci 2008, 1: 355. 10.1039/b806655hView Article
- Su P-C, Chao C-C, Shim JH, Fasching R, Prinz FB: Solid oxide fuel cell with corrugated thin film electrolyte. Nano Lett 2008, 8: 2289. 10.1021/nl800977zView Article
- Fleig J, Tuller HL, Maier J: Electrodes and electrolytes in micro-SOFCs: a discussion of geometrical constraints. Solid State Ion 2004, 174: 261. 10.1016/j.ssi.2004.07.035View Article
- Kim YB, Park JS, Gür TM, Prinz FB: Oxygen activation over engineered surface grains on YDC/YSZ interlayered composite electrolyte for LT-SOFC. J Power Sources 2011, 196: 10550. 10.1016/j.jpowsour.2011.08.075View Article
- Shim JH, Chao C-C, Huang H, Prinz FB: Atomic layer deposition of yttria-stabilized zirconia for solid oxide fuel cells. Chem Mater 2007, 19: 3850. 10.1021/cm070913tView Article
- Kerman K, Lai B-K, Ramanathan S: Pt/Y0.16Zr0.84O1.92/Pt thin film solid oxide fuel cells: electrode microstructure and stability considerations. J Power Sources 2011, 196: 2608. 10.1016/j.jpowsour.2010.10.068View Article
- Xia C, Liu M: Low-temperature SOFCs based on Gd0.1Ce0.9O1.95 fabricated by dry pressing. Solid State Ion 2001, 144: 249. 10.1016/S0167-2738(01)00980-8View Article
- Gourba E, Briois P, Ringuedé A, Cassir M, Billard A: Electrical properties of gadolinia-doped ceria thin films deposited by sputtering in view of SOFC application. J Solid State Electrochem 2004, 8: 633.View Article
- Brahim C, Ringuedé A, Gourba E, Cassir M, Billard A, Briois P: Electrical properties of thin bilayered YSZ/GDC SOFC electrolyte elaborated by sputtering. J Power Sources 2006, 194: 45.View Article
- Tsoga A, Gupta A, Naoumidis A, Nikolopoulos P: Gadolinia-doped ceria and yttria stabilized zirconia interfaces: regarding their application for SOFC technology. Acta Mater 2000, 48: 4709. 10.1016/S1359-6454(00)00261-5View Article
- Matsui T, Inaba M, Mineshige A, Ogumi Z: Electrochemical properties of ceria-based oxides for use in intermediate-temperature SOFCs. Solid State Ion 2005, 176: 647. 10.1016/j.ssi.2004.10.011View Article
- Liu QL, Khor KA, Chan SH, Chen XJ: Anode-supported solid oxide fuel cell with yttria-stabilized zirconia/gadolinia-doped ceria bilayer electrolyte prepared by wet ceramic co-sintering process. J Power Sources 2006, 162: 1036. 10.1016/j.jpowsour.2006.08.024View Article
- Duncan KL, Lee K-T, Wachsman ED: Dependence of open-circuit potential and power density on electrolyte thickness in solid oxide fuel cells with mixed conducting electrolytes. J Power Sources 2011, 196: 2445. 10.1016/j.jpowsour.2010.10.034View Article
- Myung D-H, Hong J, Yoon K, Kim B-K, Lee H-W, Lee J-H, Son J-W: The effect of an ultra-thin zirconia blocking layer on the performance of a 1-μm-thick gadolinia-doped ceria electrolyte solid-oxide fuel cell. J Power Sources 2012, 206: 91.View Article
- Cho S, Yoon J, Kim J-H, Zhang X, Manthiram A, Wang H: Microstructural and electrical properties of Ce0.9Gd0.1O1.95 thin-film electrolyte in solid-oxide fuel cells. J Mater Res 2011, 26: 854. 10.1557/jmr.2010.72View Article
- Romeo M, Bak K, Fallah JE, Normand FE, Hilaire L: XPS study of the reduction of cerium dioxide. Surf Interface Anal 1993, 20: 508. 10.1002/sia.740200604View Article
- Wibowo RA, Kim WS, Lee ES, Munir B, Kim KH: Single step preparation of quaternary Cu2ZnSnSe4 thin films by RF magnetron sputtering from binary chalcogenide targets. J Phys Chem Solids 1908, 2007: 68.
- Jiang X, Huang H, Prinz FB, Bent SF: Application of atomic layer deposition of platinum to solid oxide fuel cells. Chem Mater 2008, 20: 3897. 10.1021/cm7033189View Article
- Han J-H, Yoon D-Y: 3D CFD for chemical transport profiles in a rotating disk CVD reactor. 3D Research 2012, 2: 26.
- Liu G, Rodriguez JA, Hrbek J, Dvorak J: Electronic and chemical properties of Ce0.8Zr0.2O2(111) surfaces: photoemission, XANES, density-functional, and NO2 adsorption studies. J Phys Chem B 2001, 105: 7762. 10.1021/jp011224mView Article
- de Rouffignac P, Park J-S, Gordon RG: Atomic layer deposition of Y2O3 thin films from yttrium tris(N, N′-diisopropylacetamidinate) and water. Chem Mater 2005, 17: 4808. 10.1021/cm050624+View Article
- Kang S, Heo P, Lee YH, Ha J, Chang I, Cha S-W: Low intermediate temperature ceramic fuel cell with Y-doped BaZrO3 electrolyte and thin film Pd anode on porous substrate. Electrochem Commun 2011, 13: 374. 10.1016/j.elecom.2011.01.029View Article
- Kwon CW, Son J-W, Lee J-H, Kim H-M, Lee H-W, Kim K-B: High-performance micro-solid oxide fuel cells fabricated on nanoporous anodic aluminum oxide templates. Adv Funct Mater 2011, 18: 1154.View Article
- Kwon T-H, Lee T, Yoo H-I: Partial electronic conductivity and electrolytic domain of bilayer electrolyte Zr0.84Y0.16O1.92 /Ce0.9Gd0.1O1.95. Solid State Ion 2011, 195: 25. 10.1016/j.ssi.2011.05.002View Article
- Heo P, Kim TY, Ha J, Choi KH, Chang H, Kang S: Intermediate-temperature fuel cells with amorphous Sn0.9In0.1P2O7 thin film electrolytes. J Power Sources 2012, 198: 117.View Article
- Kwon CW, Lee J-I, Kim K-B, Lee H-W, Lee J-H, Son J-W: The thermomechanical stability of micro-solid oxide fuel cells fabricated on anodized aluminum oxide membranes. J Power Sources 2012, 210: 178.View Article
- Beckel D, Bieberle-Hütter A, Harvey A, Infortuna A, Muecke UP, Prestat M, Rupp JLM, Gauckler LJG: Thin films for micro solid oxide fuel cells. J Power Sources 2007, 173: 325. 10.1016/j.jpowsour.2007.04.070View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.